#------------------------------------------------------------------------------
#$Date: 2021-06-07 10:38:34 +0300 (Mon, 07 Jun 2021) $
#$Revision: 266209 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/31/1563178.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1563178
loop_
_publ_author_name
'Zhao, Junwei'
'Han, Qiuxia'
'Shi, Dongying'
'Chen, Lijuan'
'Ma, Pengtao'
'Wang, Jingping'
'Niu, Jingyang'
_publ_section_title
;
 Synthesis, structure and magnetism of a S-shaped multi-iron substituted
 arsenotungstate containing a trivacant Keggin [B-α-AsVW9O34]9−
 and a hexavacant Keggin [α-AsVW6O26]11− fragments
;
_journal_issue                   10
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2756
_journal_page_last               2761
_journal_paper_doi               10.1016/j.jssc.2011.08.016
_journal_volume                  184
_journal_year                    2011
_chemical_formula_sum            'C4 H52 As4 Fe8 N4 O130 W30'
_chemical_formula_weight         8498.48
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 113.05
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   30.369(11)
_cell_length_b                   21.530(10)
_cell_length_c                   11.891(5)
_cell_measurement_reflns_used    2553
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.86
_cell_measurement_theta_min      2.38
_cell_volume                     7154(5)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.971
_diffrn_measured_fraction_theta_max 0.971
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1478
_diffrn_reflns_av_sigmaI/netI    0.2262
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            17387
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.86
_exptl_absorpt_coefficient_mu    25.809
_exptl_absorpt_correction_T_max  0.0742
_exptl_absorpt_correction_T_min  0.0461
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            Brown
_exptl_crystal_density_diffrn    3.945
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Prism
_exptl_crystal_F_000             7408
_exptl_crystal_size_max          0.31
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_refine_diff_density_max         3.356
_refine_diff_density_min         -4.705
_refine_diff_density_rms         0.582
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.053
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     415
_refine_ls_number_reflns         6290
_refine_ls_number_restraints     100
_refine_ls_restrained_S_all      1.049
_refine_ls_R_factor_all          0.1897
_refine_ls_R_factor_gt           0.0970
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0522P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2098
_refine_ls_wR_factor_ref         0.2303
_reflns_number_gt                2950
_reflns_number_total             6290
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2011-184-2756.CIF
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'MULTI-SCAN' was
changed to 'multi-scan' in accordance with the built-in table derived
from the CIF Core dictionary named 'cif_core.dic' version 2.4.5 last
updated on 2014-11-21.

data item '_refine_ls_hydrogen_treatment' value 'CONSTR' was changed
to 'constr' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               1563178
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.41019(7) 0.08687(9) 0.9664(3) 0.0860(9) Uani 1 1 d . . .
W2 W 0.35098(11) 0.0000 1.1381(3) 0.0849(11) Uani 1 2 d SU . .
W3 W 0.24685(6) 0.07976(9) 0.98013(18) 0.0556(5) Uani 1 1 d . . .
W4 W 0.30536(6) 0.16572(8) 0.8107(2) 0.0652(7) Uani 1 1 d . . .
W5 W 0.35800(6) 0.08535(8) 0.6489(3) 0.0758(8) Uani 1 1 d . . .
W6 W 0.14726(5) 0.08758(7) 0.32302(15) 0.0344(4) Uani 1 1 d . . .
W7 W -0.02524(5) 0.08707(7) 0.76644(15) 0.0330(4) Uani 1 1 d . . .
W8 W -0.09495(5) 0.16822(6) 0.51640(16) 0.0375(4) Uani 1 1 d . . .
As1 As 0.3000(2) 0.0000 0.8095(8) 0.072(2) Uani 1 2 d SD . .
As2 As 0.09594(14) 0.0000 0.4994(5) 0.0215(11) Uani 1 2 d S . .
Fe1 Fe 0.2471(2) 0.0000 0.4947(8) 0.038(2) Uani 1 2 d S . .
Fe2 Fe 0.19749(15) 0.0806(2) 0.6497(5) 0.0306(12) Uani 1 1 d . . .
Fe3 Fe 0.0000 0.0781(3) 0.5000 0.0254(15) Uani 1 2 d S . .
O1W O 0.2451(14) 0.0000 0.294(4) 0.064(11) Uani 1 2 d S . .
O1 O 0.4653(12) 0.1129(15) 1.055(3) 0.093(11) Uani 1 1 d . . .
O2W O 0.240(2) 0.211(3) 0.459(6) 0.09(2) Uiso 0.50 1 d P . .
O2 O 0.3295(9) 0.0621(10) 0.813(3) 0.057(8) Uani 1 1 d . . .
O3W O 0.1235(19) 0.191(2) 0.995(5) 0.064(16) Uani 0.50 1 d PU . .
O3 O 0.3706(11) 0.1536(13) 0.943(3) 0.078(9) Uiso 1 1 d . . .
O4W O 0.281(2) 0.154(3) 0.304(6) 0.074(18) Uani 0.50 1 d PU . .
O4 O 0.4136(12) 0.0893(17) 0.816(3) 0.091(12) Uani 1 1 d . . .
O5W O 0.4849(16) 0.0000 0.807(4) 0.078(14) Uani 1 2 d S . .
O5 O 0.4249(10) 0.0000 0.917(3) 0.032(8) Uiso 1 2 d S . .
O6 O 0.3746(10) 0.0768(12) 1.084(3) 0.059 Uiso 1 1 d U . .
O7 O 0.3801(14) 0.0000 1.305(4) 0.072 Uiso 1 2 d S . .
O8 O 0.3047(11) 0.0612(13) 1.128(3) 0.088(6) Uani 1 1 d U . .
O9 O 0.2909(14) 0.0000 0.934(2) 0.068(12) Uani 1 2 d SD . .
O10 O 0.2167(10) 0.1246(13) 1.042(3) 0.078(11) Uani 1 1 d . . .
O11 O 0.2264(13) 0.0000 1.012(4) 0.059(11) Uani 1 2 d SU . .
O12 O 0.2073(9) 0.0727(10) 0.822(2) 0.050(7) Uani 1 1 d . . .
O13 O 0.2871(10) 0.1366(12) 0.938(3) 0.065(8) Uani 1 1 d . . .
O14 O 0.2489(8) 0.1403(11) 0.693(2) 0.045(7) Uani 1 1 d . . .
O15 O 0.2993(10) 0.2395(14) 0.812(3) 0.074(9) Uani 1 1 d U . .
O16 O 0.3379(9) 0.1587(13) 0.686(3) 0.080(10) Uani 1 1 d . . .
O17 O 0.3860(11) 0.1180(14) 0.568(3) 0.076(9) Uiso 1 1 d . . .
O18 O 0.3824(14) 0.0000 0.671(5) 0.075(15) Uani 1 2 d S . .
O19 O 0.2975(8) 0.0618(11) 0.542(3) 0.050(7) Uani 1 1 d U . .
O20 O 0.2473(13) 0.0000 0.687(3) 0.043(9) Uani 1 2 d S . .
O21 O 0.1947(7) 0.0672(9) 0.4809(19) 0.023(5) Uani 1 1 d U . .
O22 O 0.1488(9) 0.0000 0.623(3) 0.029(8) Uani 1 2 d S . .
O23 O 0.1816(8) 0.1152(15) 0.252(3) 0.071(9) Uani 1 1 d . . .
O24 O 0.1429(10) 0.0000 0.280(3) 0.034(8) Uani 1 2 d SU . .
O25 O 0.1364(8) 0.1615(11) 0.382(2) 0.047(7) Uani 1 1 d . . .
O26 O 0.0934(6) 0.0586(9) 0.416(2) 0.026(5) Uani 1 1 d U . .
O27 O 0.0498(12) 0.0000 0.545(3) 0.048(10) Uani 1 2 d SU . .
O28 O -0.0496(8) 0.1394(11) 0.464(2) 0.044(6) Uani 1 1 d U . .
O29 O 0.0071(7) 0.0730(8) 0.6670(18) 0.023(5) Uani 1 1 d U . .
O30 O 0.0174(8) 0.1136(10) 0.899(2) 0.038(6) Uani 1 1 d U . .
O31 O -0.0285(10) 0.0000 0.800(3) 0.028(8) Uani 1 2 d S . .
O32 O -0.0834(8) 0.0982(11) 0.797(2) 0.049(7) Uani 1 1 d U . .
O33 O -0.0447(7) 0.1639(10) 0.692(2) 0.035(6) Uani 1 1 d . . .
O34 O -0.0966(7) 0.2469(10) 0.482(2) 0.042(7) Uani 1 1 d . . .
O35 O -0.1480(9) 0.1389(11) 0.388(2) 0.052(7) Uani 1 1 d . . .
N1 N 0.0784(16) 0.0000 1.036(5) 0.08(2) Uani 1 2 d SD . .
H1C H 0.0874 0.0000 1.1164 0.125 Uiso 1 2 calc SR . .
H1D H 0.0610 -0.0338 1.0042 0.125 Uiso 0.50 1 calc PR . .
H1E H 0.0610 0.0338 1.0042 0.125 Uiso 0.50 1 calc PR . .
N2 N 0.1340(17) 0.0000 0.791(4) 0.078 Uiso 1 2 d SD . .
H2C H 0.1141 0.0000 0.7123 0.117 Uiso 1 2 calc SR . .
H2D H 0.1523 -0.0338 0.8066 0.117 Uiso 0.50 1 calc PR . .
H2E H 0.1523 0.0338 0.8066 0.117 Uiso 0.50 1 calc PR . .
C1 C 0.122(2) 0.0000 1.005(4) 0.12(3) Uiso 1 2 d SD . .
H1A H 0.1412 0.0365 1.0396 0.140 Uiso 0.50 1 calc PR . .
H1B H 0.1412 -0.0365 1.0396 0.140 Uiso 0.50 1 calc PR . .
C2 C 0.1056(15) 0.0000 0.869(4) 0.032(11) Uani 1 2 d SDU . .
H2A H 0.0848 -0.0359 0.8422 0.038 Uiso 0.50 1 calc PR . .
H2B H 0.0848 0.0359 0.8422 0.038 Uiso 0.50 1 calc PR . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O3 105.5(15) . .
O1 W1 O4 100.1(16) . .
O3 W1 O4 96.6(16) . .
O1 W1 O5 101.9(14) . .
O3 W1 O5 151.1(13) . .
O4 W1 O5 69.3(15) . .
O1 W1 O6 105.6(15) . .
O3 W1 O6 72.5(13) . .
O4 W1 O6 154.0(13) . .
O5 W1 O6 108.9(11) . .
O1 W1 O2 170.4(14) . .
O3 W1 O2 69.8(11) . .
O4 W1 O2 72.7(13) . .
O5 W1 O2 81.7(10) . .
O6 W1 O2 81.3(10) . .
O7 W2 O8 95.8(14) . 6
O7 W2 O8 95.8(14) . .
O8 W2 O8 88.1(19) 6 .
O7 W2 O6 105.5(11) . .
O8 W2 O6 154.3(12) 6 .
O8 W2 O6 75.9(13) . .
O7 W2 O6 105.5(10) . 6
O8 W2 O6 75.9(13) 6 6
O8 W2 O6 154.3(12) . 6
O6 W2 O6 111.0(16) . 6
O7 W2 O9 162.0(15) . .
O8 W2 O9 71.6(10) 6 .
O8 W2 O9 71.6(10) . .
O6 W2 O9 84.2(9) . .
O6 W2 O9 84.2(9) 6 .
O10 W3 O12 104.6(12) . .
O10 W3 O11 98.8(15) . .
O12 W3 O11 89.8(14) . .
O10 W3 O13 104.9(13) . .
O12 W3 O13 90.8(12) . .
O11 W3 O13 155.4(13) . .
O10 W3 O8 99.9(14) . .
O12 W3 O8 155.2(13) . .
O11 W3 O8 83.5(15) . .
O13 W3 O8 85.7(13) . .
O10 W3 O9 165.7(11) . .
O12 W3 O9 84.4(11) . .
O11 W3 O9 69.7(12) . .
O13 W3 O9 85.8(9) . .
O8 W3 O9 71.0(13) . .
O15 W4 O14 103.2(12) . .
O15 W4 O13 104.5(15) . .
O14 W4 O13 91.8(12) . .
O15 W4 O3 101.8(13) . .
O14 W4 O3 155.0(11) . .
O13 W4 O3 80.7(13) . .
O15 W4 O16 99.5(15) . .
O14 W4 O16 89.9(12) . .
O13 W4 O16 154.9(11) . .
O3 W4 O16 87.3(12) . .
O15 W4 O2 168.7(12) . .
O14 W4 O2 85.3(10) . .
O13 W4 O2 82.4(11) . .
O3 W4 O2 70.2(10) . .
O16 W4 O2 72.8(11) . .
O17 W5 O16 93.9(15) . .
O17 W5 O19 108.4(13) . .
O16 W5 O19 93.8(12) . .
O17 W5 O18 102.9(15) . .
O16 W5 O18 158.7(18) . .
O19 W5 O18 93.3(15) . .
O17 W5 O4 97.2(14) . .
O16 W5 O4 87.5(15) . .
O19 W5 O4 154.1(13) . .
O18 W5 O4 77.5(18) . .
O17 W5 O2 162.5(12) . .
O16 W5 O2 74.4(12) . .
O19 W5 O2 85.6(10) . .
O18 W5 O2 86.2(14) . .
O4 W5 O2 69.8(11) . .
O23 W6 O25 97.2(13) . .
O23 W6 O21 101.2(11) . .
O25 W6 O21 90.1(10) . .
O23 W6 O32 103.3(12) . 2_556
O25 W6 O32 84.3(11) . 2_556
O21 W6 O32 155.4(10) . 2_556
O23 W6 O24 101.8(14) . .
O25 W6 O24 160.8(11) . .
O21 W6 O24 89.0(11) . .
O32 W6 O24 88.6(11) 2_556 .
O23 W6 O26 173.7(10) . .
O25 W6 O26 77.9(8) . .
O21 W6 O26 82.9(8) . .
O32 W6 O26 72.5(9) 2_556 .
O24 W6 O26 83.0(10) . .
O30 W7 O29 104.2(10) . .
O30 W7 O33 97.2(10) . .
O29 W7 O33 89.6(9) . .
O30 W7 O31 102.6(12) . .
O29 W7 O31 93.3(10) . .
O33 W7 O31 158.6(11) . .
O30 W7 O32 101.7(11) . .
O29 W7 O32 153.2(10) . .
O33 W7 O32 80.5(9) . .
O31 W7 O32 87.5(10) . .
O30 W7 O26 172.1(9) . 2_556
O29 W7 O26 82.4(8) . 2_556
O33 W7 O26 78.4(8) . 2_556
O31 W7 O26 81.0(11) . 2_556
O32 W7 O26 71.2(9) . 2_556
O34 W8 O28 102.0(11) . .
O34 W8 O35 101.8(11) . .
O28 W8 O35 97.5(12) . .
O34 W8 O33 102.9(10) . .
O28 W8 O33 88.6(10) . .
O35 W8 O33 152.6(10) . .
O34 W8 O25 103.7(10) . 2_556
O28 W8 O25 152.9(10) . 2_556
O35 W8 O25 85.7(11) . 2_556
O33 W8 O25 77.3(9) . 2_556
O34 W8 O26 174.3(10) . 2_556
O28 W8 O26 82.5(9) . 2_556
O35 W8 O26 81.0(9) . 2_556
O33 W8 O26 73.4(8) . 2_556
O25 W8 O26 71.4(8) 2_556 2_556
O2 As1 O2 113.2(18) . 6
O2 As1 O9 106.0(13) . .
O2 As1 O9 106.0(13) 6 .
O2 As1 O20 110.7(11) . .
O2 As1 O20 110.7(12) 6 .
O9 As1 O20 110.2(19) . .
O26 As2 O26 104.9(15) 6 .
O26 As2 O27 111.0(10) 6 .
O26 As2 O27 111.0(10) . .
O26 As2 O22 109.8(9) 6 .
O26 As2 O22 109.8(9) . .
O27 As2 O22 110.2(16) . .
O19 Fe1 O19 86.7(15) . 6
O19 Fe1 O21 168.3(11) . 6
O19 Fe1 O21 92.1(9) 6 6
O19 Fe1 O21 92.1(9) . .
O19 Fe1 O21 168.3(11) 6 .
O21 Fe1 O21 86.7(11) 6 .
O19 Fe1 O20 90.8(11) . .
O19 Fe1 O20 90.8(11) 6 .
O21 Fe1 O20 77.5(9) 6 .
O21 Fe1 O20 77.5(9) . .
O19 Fe1 O1W 90.1(11) . .
O19 Fe1 O1W 90.1(11) 6 .
O21 Fe1 O1W 101.6(9) 6 .
O21 Fe1 O1W 101.6(9) . .
O20 Fe1 O1W 178.8(13) . .
O35 Fe2 O14 96.2(12) 2_556 .
O35 Fe2 O12 95.1(11) 2_556 .
O14 Fe2 O12 90.1(10) . .
O35 Fe2 O21 98.1(10) 2_556 .
O14 Fe2 O21 94.4(10) . .
O12 Fe2 O21 165.5(9) . .
O35 Fe2 O22 93.5(10) 2_556 .
O14 Fe2 O22 169.2(9) . .
O12 Fe2 O22 84.5(11) . .
O21 Fe2 O22 88.8(10) . .
O35 Fe2 O20 170.9(11) 2_556 .
O14 Fe2 O20 92.9(10) . .
O12 Fe2 O20 84.8(12) . .
O21 Fe2 O20 81.3(10) . .
O22 Fe2 O20 77.4(9) . .
O29 Fe3 O29 173.5(11) . 2_556
O29 Fe3 O28 92.6(10) . 2_556
O29 Fe3 O28 91.9(9) 2_556 2_556
O29 Fe3 O28 91.9(9) . .
O29 Fe3 O28 92.6(10) 2_556 .
O28 Fe3 O28 93.2(14) 2_556 .
O29 Fe3 O27 89.8(12) . 5_556
O29 Fe3 O27 85.2(11) 2_556 5_556
O28 Fe3 O27 172.5(10) 2_556 5_556
O28 Fe3 O27 93.8(10) . 5_556
O29 Fe3 O27 85.2(11) . .
O29 Fe3 O27 89.8(12) 2_556 .
O28 Fe3 O27 93.8(10) 2_556 .
O28 Fe3 O27 172.5(10) . .
O27 Fe3 O27 79.3(14) 5_556 .
As1 O2 W4 128.6(14) . .
As1 O2 W5 121.1(15) . .
W4 O2 W5 90.3(9) . .
As1 O2 W1 125.4(14) . .
W4 O2 W1 91.0(8) . .
W5 O2 W1 89.3(9) . .
W1 O3 W4 127.6(17) . .
W1 O4 W5 127.3(18) . .
W1 O5 W1 130.3(16) 6 .
W2 O6 W1 130.2(14) . .
W2 O8 W3 125.3(18) . .
As1 O9 W3 122.0(10) . 6
As1 O9 W3 122.0(10) . .
W3 O9 W3 92.8(9) 6 .
As1 O9 W2 127(2) . .
W3 O9 W2 92.2(5) 6 .
W3 O9 W2 92.2(5) . .
W3 O11 W3 128(2) . 6
W3 O12 Fe2 148.6(15) . .
W4 O13 W3 145.3(17) . .
W4 O14 Fe2 145.7(14) . .
W5 O16 W4 122.3(16) . .
W5 O18 W5 139(2) . 6
W5 O19 Fe1 148.1(15) . .
As1 O20 Fe2 120.9(10) . 6
As1 O20 Fe2 120.9(10) . .
Fe2 O20 Fe2 102.3(14) 6 .
As1 O20 Fe1 119.4(18) . .
Fe2 O20 Fe1 93.6(11) 6 .
Fe2 O20 Fe1 93.6(11) . .
W6 O21 Fe2 132.1(9) . .
W6 O21 Fe1 119.2(10) . .
Fe2 O21 Fe1 106.7(9) . .
As2 O22 Fe2 118.4(10) . .
As2 O22 Fe2 118.4(10) . 6
Fe2 O22 Fe2 102.8(11) . 6
W6 O24 W6 151.9(18) 6 .
W6 O25 W8 122.1(11) . 2_556
As2 O26 W6 128.6(10) . .
As2 O26 W7 125.2(10) . 2_556
W6 O26 W7 91.3(7) . 2_556
As2 O26 W8 123.9(11) . 2_556
W6 O26 W8 88.4(6) . 2_556
W7 O26 W8 87.2(6) 2_556 2_556
As2 O27 Fe3 120.3(11) . 5_556
As2 O27 Fe3 120.3(11) . .
Fe3 O27 Fe3 100.7(14) 5_556 .
W8 O28 Fe3 141.7(15) . .
W7 O29 Fe3 142.0(11) . .
W7 O31 W7 153.1(17) . 6
W6 O32 W7 124.8(14) 2_556 .
W7 O33 W8 119.7(11) . .
W8 O35 Fe2 141.9(15) . 2_556
C1 N1 H1C 109.5 . .
C1 N1 H1D 109.5 . .
H1C N1 H1D 109.5 . .
C1 N1 H1E 109.5 . .
H1C N1 H1E 109.5 . .
H1D N1 H1E 109.5 . .
C2 N2 H2C 109.5 . .
C2 N2 H2D 109.5 . .
H2C N2 H2D 109.5 . .
C2 N2 H2E 109.5 . .
H2C N2 H2E 109.5 . .
H2D N2 H2E 109.5 . .
C2 C1 N1 108(5) . .
C2 C1 H1A 110.1 . .
N1 C1 H1A 110.1 . .
C2 C1 H1B 110.1 . .
N1 C1 H1B 110.1 . .
H1A C1 H1B 108.4 . .
N2 C2 C1 130(4) . .
N2 C2 H2A 104.7 . .
C1 C2 H2A 104.7 . .
N2 C2 H2B 104.7 . .
C1 C2 H2B 104.7 . .
H2A C2 H2B 105.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O1 1.69(3) .
W1 O3 1.83(3) .
W1 O4 1.84(3) .
W1 O5 2.061(14) .
W1 O6 2.08(3) .
W1 O2 2.47(3) .
W2 O7 1.83(4) .
W2 O8 1.89(3) 6
W2 O8 1.89(3) .
W2 O6 2.01(3) .
W2 O6 2.01(3) 6
W2 O9 2.40(3) .
W3 O10 1.69(3) .
W3 O12 1.80(2) .
W3 O11 1.914(18) .
W3 O13 1.93(3) .
W3 O8 1.98(3) .
W3 O9 2.372(19) .
W4 O15 1.60(3) .
W4 O14 1.82(2) .
W4 O13 1.92(3) .
W4 O3 2.01(3) .
W4 O16 2.09(3) .
W4 O2 2.34(2) .
W5 O17 1.66(3) .
W5 O16 1.81(3) .
W5 O19 1.85(2) .
W5 O18 1.960(13) .
W5 O4 2.04(3) .
W5 O2 2.47(3) .
W6 O23 1.68(3) .
W6 O25 1.82(3) .
W6 O21 1.917(19) .
W6 O32 1.92(2) 2_556
W6 O24 1.944(8) .
W6 O26 2.384(19) .
W7 O30 1.70(2) .
W7 O29 1.83(2) .
W7 O33 1.86(2) .
W7 O31 1.927(7) .
W7 O32 1.95(2) .
W7 O26 2.42(2) 2_556
W8 O34 1.74(2) .
W8 O28 1.83(2) .
W8 O35 1.84(2) .
W8 O33 2.05(2) .
W8 O25 2.06(2) 2_556
W8 O26 2.49(2) 2_556
As1 O2 1.60(2) .
As1 O2 1.60(2) 6
As1 O9 1.605(10) .
As1 O20 1.69(4) .
As2 O26 1.59(2) 6
As2 O26 1.59(2) .
As2 O27 1.69(4) .
As2 O22 1.70(3) .
Fe1 O19 1.94(2) .
Fe1 O19 1.94(2) 6
Fe1 O21 2.109(18) 6
Fe1 O21 2.109(18) .
Fe1 O20 2.29(3) .
Fe1 O1W 2.36(4) .
Fe2 O35 1.87(2) 2_556
Fe2 O14 1.93(2) .
Fe2 O12 1.95(3) .
Fe2 O21 2.00(2) .
Fe2 O22 2.221(17) .
Fe2 O20 2.23(2) .
Fe3 O29 1.91(2) .
Fe3 O29 1.91(2) 2_556
Fe3 O28 1.92(2) 2_556
Fe3 O28 1.92(2) .
Fe3 O27 2.18(2) 5_556
Fe3 O27 2.18(2) .
O5 W1 2.061(14) 6
O9 W3 2.372(19) 6
O11 W3 1.914(18) 6
O18 W5 1.960(13) 6
O20 Fe2 2.23(2) 6
O22 Fe2 2.221(17) 6
O24 W6 1.944(8) 6
O25 W8 2.06(2) 2_556
O26 W7 2.42(2) 2_556
O26 W8 2.49(2) 2_556
O27 Fe3 2.18(2) 5_556
O31 W7 1.927(7) 6
O32 W6 1.92(2) 2_556
O35 Fe2 1.87(2) 2_556
N1 C1 1.498(10) .
N1 H1C 0.8900 .
N1 H1D 0.8900 .
N1 H1E 0.8900 .
N2 C2 1.497(10) .
N2 H2C 0.8900 .
N2 H2D 0.8900 .
N2 H2E 0.8900 .
C1 C2 1.497(10) .
C1 H1A 0.9700 .
C1 H1B 0.9700 .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
O2 As1 O2 W4 -179.8(3) 6 . . .
O9 As1 O2 W4 -64(2) . . . .
O20 As1 O2 W4 55(2) . . . .
O2 As1 O2 W5 61(3) 6 . . .
O9 As1 O2 W5 176.7(16) . . . .
O20 As1 O2 W5 -63.9(18) . . . .
O2 As1 O2 W1 -53(3) 6 . . .
O9 As1 O2 W1 62(2) . . . .
O20 As1 O2 W1 -178.2(16) . . . .
O15 W4 O2 As1 178(6) . . . .
O14 W4 O2 As1 -43(2) . . . .
O13 W4 O2 As1 49(2) . . . .
O3 W4 O2 As1 132(2) . . . .
O16 W4 O2 As1 -135(2) . . . .
O15 W4 O2 W5 -51(7) . . . .
O14 W4 O2 W5 88.4(10) . . . .
O13 W4 O2 W5 -179.2(11) . . . .
O3 W4 O2 W5 -96.4(12) . . . .
O16 W4 O2 W5 -3.0(9) . . . .
O15 W4 O2 W1 39(7) . . . .
O14 W4 O2 W1 177.7(11) . . . .
O13 W4 O2 W1 -89.8(11) . . . .
O3 W4 O2 W1 -7.0(12) . . . .
O16 W4 O2 W1 86.4(11) . . . .
O17 W5 O2 As1 -171(3) . . . .
O16 W5 O2 As1 140.4(18) . . . .
O19 W5 O2 As1 45.2(16) . . . .
O18 W5 O2 As1 -48.4(18) . . . .
O4 W5 O2 As1 -126.5(19) . . . .
O17 W5 O2 W4 52(4) . . . .
O16 W5 O2 W4 3.4(10) . . . .
O19 W5 O2 W4 -91.8(10) . . . .
O18 W5 O2 W4 174.6(14) . . . .
O4 W5 O2 W4 96.6(13) . . . .
O17 W5 O2 W1 -39(4) . . . .
O16 W5 O2 W1 -87.6(11) . . . .
O19 W5 O2 W1 177.2(10) . . . .
O18 W5 O2 W1 83.6(14) . . . .
O4 W5 O2 W1 5.6(12) . . . .
O1 W1 O2 As1 165(8) . . . .
O3 W1 O2 As1 -133(2) . . . .
O4 W1 O2 As1 123(2) . . . .
O5 W1 O2 As1 51.8(18) . . . .
O6 W1 O2 As1 -58.9(18) . . . .
O1 W1 O2 W4 -54(8) . . . .
O3 W1 O2 W4 7.8(13) . . . .
O4 W1 O2 W4 -96.4(15) . . . .
O5 W1 O2 W4 -167.2(12) . . . .
O6 W1 O2 W4 82.2(10) . . . .
O1 W1 O2 W5 36(8) . . . .
O3 W1 O2 W5 98.0(13) . . . .
O4 W1 O2 W5 -6.1(13) . . . .
O5 W1 O2 W5 -76.9(10) . . . .
O6 W1 O2 W5 172.4(9) . . . .
O1 W1 O3 W4 160(2) . . . .
O4 W1 O3 W4 57(2) . . . .
O5 W1 O3 W4 -1(4) . . . .
O6 W1 O3 W4 -99(2) . . . .
O2 W1 O3 W4 -11.5(18) . . . .
O15 W4 O3 W1 -160(2) . . . .
O14 W4 O3 W1 23(5) . . . .
O13 W4 O3 W1 97(2) . . . .
O16 W4 O3 W1 -61(2) . . . .
O2 W4 O3 W1 12.1(19) . . . .
O1 W1 O4 W5 -164(2) . . . .
O3 W1 O4 W5 -57(2) . . . .
O5 W1 O4 W5 97(2) . . . .
O6 W1 O4 W5 6(5) . . . .
O2 W1 O4 W5 9.3(19) . . . .
O17 W5 O4 W1 158(2) . . . .
O16 W5 O4 W1 65(2) . . . .
O19 W5 O4 W1 -29(5) . . . .
O18 W5 O4 W1 -100(3) . . . .
O2 W5 O4 W1 -9(2) . . . .
O1 W1 O5 W1 111(2) . . . 6
O3 W1 O5 W1 -88(3) . . . 6
O4 W1 O5 W1 -153(2) . . . 6
O6 W1 O5 W1 0(2) . . . 6
O2 W1 O5 W1 -78.3(19) . . . 6
O7 W2 O6 W1 123(2) . . . .
O8 W2 O6 W1 -92(3) 6 . . .
O8 W2 O6 W1 -145(2) . . . .
O6 W2 O6 W1 9(3) 6 . . .
O9 W2 O6 W1 -72.8(17) . . . .
O1 W1 O6 W2 -114(2) . . . .
O3 W1 O6 W2 145(2) . . . .
O4 W1 O6 W2 77(4) . . . .
O5 W1 O6 W2 -5(2) . . . .
O2 W1 O6 W2 73.3(17) . . . .
O7 W2 O8 W3 -166(2) . . . .
O8 W2 O8 W3 -70(3) 6 . . .
O6 W2 O8 W3 90(2) . . . .
O6 W2 O8 W3 -20(5) 6 . . .
O9 W2 O8 W3 1.0(17) . . . .
O10 W3 O8 W2 168(2) . . . .
O12 W3 O8 W2 -6(5) . . . .
O11 W3 O8 W2 70(2) . . . .
O13 W3 O8 W2 -88(2) . . . .
O9 W3 O8 W2 -1.0(17) . . . .
O2 As1 O9 W3 178.4(16) . . . 6
O2 As1 O9 W3 -61(2) 6 . . 6
O20 As1 O9 W3 58.6(17) . . . 6
O2 As1 O9 W3 61(2) . . . .
O2 As1 O9 W3 -178.4(16) 6 . . .
O20 As1 O9 W3 -58.6(17) . . . .
O2 As1 O9 W2 -60.2(10) . . . .
O2 As1 O9 W2 60.2(10) 6 . . .
O20 As1 O9 W2 180.000(2) . . . .
O10 W3 O9 As1 172(4) . . . .
O12 W3 O9 As1 42(2) . . . .
O11 W3 O9 As1 134(3) . . . .
O13 W3 O9 As1 -49(2) . . . .
O8 W3 O9 As1 -136(2) . . . .
O10 W3 O9 W3 41(5) . . . 6
O12 W3 O9 W3 -88.9(11) . . . 6
O11 W3 O9 W3 3.0(13) . . . 6
O13 W3 O9 W3 179.8(12) . . . 6
O8 W3 O9 W3 93.0(13) . . . 6
O10 W3 O9 W2 -52(5) . . . .
O12 W3 O9 W2 178.7(9) . . . .
O11 W3 O9 W2 -89.4(13) . . . .
O13 W3 O9 W2 87.5(10) . . . .
O8 W3 O9 W2 0.6(11) . . . .
O7 W2 O9 As1 180.000(10) . . . .
O8 W2 O9 As1 -132.9(11) 6 . . .
O8 W2 O9 As1 132.9(11) . . . .
O6 W2 O9 As1 55.9(8) . . . .
O6 W2 O9 As1 -55.9(8) 6 . . .
O7 W2 O9 W3 -46.4(5) . . . 6
O8 W2 O9 W3 0.7(11) 6 . . 6
O8 W2 O9 W3 -93.5(13) . . . 6
O6 W2 O9 W3 -170.5(10) . . . 6
O6 W2 O9 W3 77.7(9) 6 . . 6
O7 W2 O9 W3 46.4(5) . . . .
O8 W2 O9 W3 93.5(13) 6 . . .
O8 W2 O9 W3 -0.7(11) . . . .
O6 W2 O9 W3 -77.7(9) . . . .
O6 W2 O9 W3 170.5(10) 6 . . .
O10 W3 O11 W3 -176(2) . . . 6
O12 W3 O11 W3 79(3) . . . 6
O13 W3 O11 W3 -12(5) . . . 6
O8 W3 O11 W3 -77(3) . . . 6
O9 W3 O11 W3 -5(2) . . . 6
O10 W3 O12 Fe2 127(3) . . . .
O11 W3 O12 Fe2 -134(3) . . . .
O13 W3 O12 Fe2 22(3) . . . .
O8 W3 O12 Fe2 -60(4) . . . .
O9 W3 O12 Fe2 -64(3) . . . .
O35 Fe2 O12 W3 -120(3) 2_556 . . .
O14 Fe2 O12 W3 -24(3) . . . .
O21 Fe2 O12 W3 84(4) . . . .
O22 Fe2 O12 W3 146(3) . . . .
O20 Fe2 O12 W3 69(3) . . . .
O15 W4 O13 W3 128(2) . . . .
O14 W4 O13 W3 24(2) . . . .
O3 W4 O13 W3 -132(3) . . . .
O16 W4 O13 W3 -70(4) . . . .
O2 W4 O13 W3 -61(2) . . . .
O10 W3 O13 W4 -126(2) . . . .
O12 W3 O13 W4 -21(3) . . . .
O11 W3 O13 W4 71(5) . . . .
O8 W3 O13 W4 135(3) . . . .
O9 W3 O13 W4 64(2) . . . .
O15 W4 O14 Fe2 -135(3) . . . .
O13 W4 O14 Fe2 -30(3) . . . .
O3 W4 O14 Fe2 42(5) . . . .
O16 W4 O14 Fe2 125(3) . . . .
O2 W4 O14 Fe2 52(3) . . . .
O35 Fe2 O14 W4 125(3) 2_556 . . .
O12 Fe2 O14 W4 30(3) . . . .
O21 Fe2 O14 W4 -137(3) . . . .
O22 Fe2 O14 W4 -30(8) . . . .
O20 Fe2 O14 W4 -55(3) . . . .
O17 W5 O16 W4 -171.4(18) . . . .
O19 W5 O16 W4 79.8(18) . . . .
O18 W5 O16 W4 -29(5) . . . .
O4 W5 O16 W4 -74.3(18) . . . .
O2 W5 O16 W4 -4.5(14) . . . .
O15 W4 O16 W5 176.4(18) . . . .
O14 W4 O16 W5 -80.3(17) . . . .
O13 W4 O16 W5 14(4) . . . .
O3 W4 O16 W5 74.9(18) . . . .
O2 W4 O16 W5 4.8(15) . . . .
O17 W5 O18 W5 -129(4) . . . 6
O16 W5 O18 W5 90(6) . . . 6
O19 W5 O18 W5 -19(4) . . . 6
O4 W5 O18 W5 136(4) . . . 6
O2 W5 O18 W5 66(4) . . . 6
O17 W5 O19 Fe1 138(3) . . . .
O16 W5 O19 Fe1 -126(3) . . . .
O18 W5 O19 Fe1 34(3) . . . .
O4 W5 O19 Fe1 -34(5) . . . .
O2 W5 O19 Fe1 -52(3) . . . .
O19 Fe1 O19 W5 -37(3) 6 . . .
O21 Fe1 O19 W5 48(6) 6 . . .
O21 Fe1 O19 W5 132(3) . . . .
O20 Fe1 O19 W5 54(3) . . . .
O1W Fe1 O19 W5 -127(3) . . . .
O2 As1 O20 Fe2 178.0(16) . . . 6
O2 As1 O20 Fe2 52(2) 6 . . 6
O9 As1 O20 Fe2 -65.1(16) . . . 6
O2 As1 O20 Fe2 -52(2) . . . .
O2 As1 O20 Fe2 -178.0(16) 6 . . .
O9 As1 O20 Fe2 65.1(16) . . . .
O2 As1 O20 Fe1 63.1(12) . . . .
O2 As1 O20 Fe1 -63.1(12) 6 . . .
O9 As1 O20 Fe1 180.000(3) . . . .
O35 Fe2 O20 As1 -139(7) 2_556 . . .
O14 Fe2 O20 As1 40.5(19) . . . .
O12 Fe2 O20 As1 -49.3(18) . . . .
O21 Fe2 O20 As1 134.5(19) . . . .
O22 Fe2 O20 As1 -135(2) . . . .
O35 Fe2 O20 Fe2 -1(8) 2_556 . . 6
O14 Fe2 O20 Fe2 178.4(13) . . . 6
O12 Fe2 O20 Fe2 88.6(13) . . . 6
O21 Fe2 O20 Fe2 -87.6(12) . . . 6
O22 Fe2 O20 Fe2 3.1(12) . . . 6
O35 Fe2 O20 Fe1 94(8) 2_556 . . .
O14 Fe2 O20 Fe1 -87.1(11) . . . .
O12 Fe2 O20 Fe1 -176.9(11) . . . .
O21 Fe2 O20 Fe1 6.9(9) . . . .
O22 Fe2 O20 Fe1 97.6(12) . . . .
O19 Fe1 O20 As1 -43.3(7) . . . .
O19 Fe1 O20 As1 43.3(7) 6 . . .
O21 Fe1 O20 As1 135.3(6) 6 . . .
O21 Fe1 O20 As1 -135.3(6) . . . .
O1W Fe1 O20 As1 180.00(13) . . . .
O19 Fe1 O20 Fe2 -172.1(10) . . . 6
O19 Fe1 O20 Fe2 -85.4(11) 6 . . 6
O21 Fe1 O20 Fe2 6.6(9) 6 . . 6
O21 Fe1 O20 Fe2 95.9(10) . . . 6
O1W Fe1 O20 Fe2 51.3(8) . . . 6
O19 Fe1 O20 Fe2 85.4(11) . . . .
O19 Fe1 O20 Fe2 172.1(10) 6 . . .
O21 Fe1 O20 Fe2 -95.9(10) 6 . . .
O21 Fe1 O20 Fe2 -6.6(9) . . . .
O1W Fe1 O20 Fe2 -51.3(8) . . . .
O23 W6 O21 Fe2 136.8(17) . . . .
O25 W6 O21 Fe2 39.5(15) . . . .
O32 W6 O21 Fe2 -37(3) 2_556 . . .
O24 W6 O21 Fe2 -121.4(16) . . . .
O26 W6 O21 Fe2 -38.3(14) . . . .
O23 W6 O21 Fe1 -61.5(15) . . . .
O25 W6 O21 Fe1 -158.8(12) . . . .
O32 W6 O21 Fe1 125(2) 2_556 . . .
O24 W6 O21 Fe1 40.4(13) . . . .
O26 W6 O21 Fe1 123.4(11) . . . .
O35 Fe2 O21 W6 -15.2(17) 2_556 . . .
O14 Fe2 O21 W6 -112.1(15) . . . .
O12 Fe2 O21 W6 140(3) . . . .
O22 Fe2 O21 W6 78.2(15) . . . .
O20 Fe2 O21 W6 155.6(16) . . . .
O35 Fe2 O21 Fe1 -178.6(11) 2_556 . . .
O14 Fe2 O21 Fe1 84.4(10) . . . .
O12 Fe2 O21 Fe1 -23(4) . . . .
O22 Fe2 O21 Fe1 -85.2(9) . . . .
O20 Fe2 O21 Fe1 -7.8(10) . . . .
O19 Fe1 O21 W6 111.3(13) . . . .
O19 Fe1 O21 W6 -165(4) 6 . . .
O21 Fe1 O21 W6 -80.3(13) 6 . . .
O20 Fe1 O21 W6 -158.3(13) . . . .
O1W Fe1 O21 W6 20.8(13) . . . .
O19 Fe1 O21 Fe2 -82.7(12) . . . .
O19 Fe1 O21 Fe2 1(5) 6 . . .
O21 Fe1 O21 Fe2 85.6(10) 6 . . .
O20 Fe1 O21 Fe2 7.7(10) . . . .
O1W Fe1 O21 Fe2 -173.2(9) . . . .
O26 As2 O22 Fe2 120.1(12) 6 . . .
O26 As2 O22 Fe2 5.2(17) . . . .
O27 As2 O22 Fe2 -117.3(12) . . . .
O26 As2 O22 Fe2 -5.2(17) 6 . . 6
O26 As2 O22 Fe2 -120.1(12) . . . 6
O27 As2 O22 Fe2 117.3(12) . . . 6
O35 Fe2 O22 As2 43.7(16) 2_556 . . .
O14 Fe2 O22 As2 -162(5) . . . .
O12 Fe2 O22 As2 138.4(15) . . . .
O21 Fe2 O22 As2 -54.4(14) . . . .
O20 Fe2 O22 As2 -135.7(17) . . . .
O35 Fe2 O22 Fe2 176.3(13) 2_556 . . 6
O14 Fe2 O22 Fe2 -29(7) . . . 6
O12 Fe2 O22 Fe2 -89.0(13) . . . 6
O21 Fe2 O22 Fe2 78.2(11) . . . 6
O20 Fe2 O22 Fe2 -3.1(12) . . . 6
O23 W6 O24 W6 131(3) . . . 6
O25 W6 O24 W6 -58(6) . . . 6
O21 W6 O24 W6 29(3) . . . 6
O32 W6 O24 W6 -126(3) 2_556 . . 6
O26 W6 O24 W6 -54(3) . . . 6
O23 W6 O25 W8 179.6(15) . . . 2_556
O21 W6 O25 W8 -79.1(14) . . . 2_556
O32 W6 O25 W8 76.9(15) 2_556 . . 2_556
O24 W6 O25 W8 8(5) . . . 2_556
O26 W6 O25 W8 3.6(12) . . . 2_556
O26 As2 O26 W6 -60.7(18) 6 . . .
O27 As2 O26 W6 179.3(15) . . . .
O22 As2 O26 W6 57.2(17) . . . .
O26 As2 O26 W7 65.9(16) 6 . . 2_556
O27 As2 O26 W7 -54.1(17) . . . 2_556
O22 As2 O26 W7 -176.2(12) . . . 2_556
O26 As2 O26 W8 179.59(13) 6 . . 2_556
O27 As2 O26 W8 59.6(16) . . . 2_556
O22 As2 O26 W8 -62.5(14) . . . 2_556
O23 W6 O26 As2 -175(11) . . . .
O25 W6 O26 As2 -136.4(17) . . . .
O21 W6 O26 As2 -44.8(15) . . . .
O32 W6 O26 As2 135.8(17) 2_556 . . .
O24 W6 O26 As2 45.1(16) . . . .
O23 W6 O26 W7 45(11) . . . 2_556
O25 W6 O26 W7 84.6(9) . . . 2_556
O21 W6 O26 W7 176.2(8) . . . 2_556
O32 W6 O26 W7 -3.2(8) 2_556 . . 2_556
O24 W6 O26 W7 -93.9(10) . . . 2_556
O23 W6 O26 W8 -42(11) . . . 2_556
O25 W6 O26 W8 -2.5(9) . . . 2_556
O21 W6 O26 W8 89.1(7) . . . 2_556
O32 W6 O26 W8 -90.3(9) 2_556 . . 2_556
O24 W6 O26 W8 178.9(10) . . . 2_556
O26 As2 O27 Fe3 5(2) 6 . . 5_556
O26 As2 O27 Fe3 121.3(14) . . . 5_556
O22 As2 O27 Fe3 -116.9(16) . . . 5_556
O26 As2 O27 Fe3 -121.3(14) 6 . . .
O26 As2 O27 Fe3 -5(2) . . . .
O22 As2 O27 Fe3 116.9(16) . . . .
O29 Fe3 O27 As2 -134.5(19) . . . .
O29 Fe3 O27 As2 49.6(18) 2_556 . . .
O28 Fe3 O27 As2 -42.2(19) 2_556 . . .
O28 Fe3 O27 As2 158(8) . . . .
O27 Fe3 O27 As2 135(3) 5_556 . . .
O29 Fe3 O27 Fe3 90.7(13) . . . 5_556
O29 Fe3 O27 Fe3 -85.2(13) 2_556 . . 5_556
O28 Fe3 O27 Fe3 -177.1(13) 2_556 . . 5_556
O28 Fe3 O27 Fe3 23(10) . . . 5_556
O27 Fe3 O27 Fe3 0.000(1) 5_556 . . 5_556
O34 W8 O28 Fe3 147(2) . . . .
O35 W8 O28 Fe3 -109(2) . . . .
O33 W8 O28 Fe3 44(2) . . . .
O25 W8 O28 Fe3 -14(4) 2_556 . . .
O26 W8 O28 Fe3 -29(2) 2_556 . . .
O29 Fe3 O28 W8 -24(2) . . . .
O29 Fe3 O28 W8 152(2) 2_556 . . .
O28 Fe3 O28 W8 -116(2) 2_556 . . .
O27 Fe3 O28 W8 66(2) 5_556 . . .
O27 Fe3 O28 W8 44(10) . . . .
O30 W7 O29 Fe3 -144.1(17) . . . .
O33 W7 O29 Fe3 -46.7(18) . . . .
O31 W7 O29 Fe3 112.0(19) . . . .
O32 W7 O29 Fe3 21(3) . . . .
O26 W7 O29 Fe3 31.6(17) 2_556 . . .
O29 Fe3 O29 W7 -109.9(17) 2_556 . . .
O28 Fe3 O29 W7 116.7(18) 2_556 . . .
O28 Fe3 O29 W7 23.5(19) . . . .
O27 Fe3 O29 W7 -70.4(18) 5_556 . . .
O27 Fe3 O29 W7 -149.6(19) . . . .
O30 W7 O31 W7 -123(4) . . . 6
O29 W7 O31 W7 -18(4) . . . 6
O33 W7 O31 W7 80(5) . . . 6
O32 W7 O31 W7 135(4) . . . 6
O26 W7 O31 W7 64(4) 2_556 . . 6
O30 W7 O32 W6 171.5(14) . . . 2_556
O29 W7 O32 W6 6(3) . . . 2_556
O33 W7 O32 W6 76.1(15) . . . 2_556
O31 W7 O32 W6 -86.1(17) . . . 2_556
O26 W7 O32 W6 -4.8(12) 2_556 . . 2_556
O30 W7 O33 W8 175.8(12) . . . .
O29 W7 O33 W8 71.6(12) . . . .
O31 W7 O33 W8 -27(4) . . . .
O32 W7 O33 W8 -83.4(13) . . . .
O26 W7 O33 W8 -10.8(10) 2_556 . . .
O34 W8 O33 W7 -173.8(12) . . . .
O28 W8 O33 W7 -71.8(13) . . . .
O35 W8 O33 W7 32(3) . . . .
O25 W8 O33 W7 84.8(12) 2_556 . . .
O26 W8 O33 W7 10.7(10) 2_556 . . .
O34 W8 O35 Fe2 -144(3) . . . 2_556
O28 W8 O35 Fe2 112(3) . . . 2_556
O33 W8 O35 Fe2 10(4) . . . 2_556
O25 W8 O35 Fe2 -41(3) 2_556 . . 2_556
O26 W8 O35 Fe2 31(2) 2_556 . . 2_556
N1 C1 C2 N2 180.000(14) . . . .
